# Assignment 5 solutions ```MAE 20
Winter 2011
Assignment 5
6.7 For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the
modulus of elasticity is 115 GPa (16.7 &times; 106 psi).
(a) What is the maximum load that may be applied to a specimen with a cross-sectional area of 325 mm2
(0.5 in.2) without plastic deformation?
(b) If the original specimen length is 115 mm (4.5 in.), what is the maximum length to which it may be
stretched without causing plastic deformation?
Solution
(a) This portion of the problem calls for a determination of the maximum load that can be applied without
plastic deformation (Fy). Taking the yield strength to be 275 MPa, and employment of Equation 6.1 leads to
Fy = ! y A0 = (275 &quot; 10 6 N/m2 )(325 &quot; 10 -6 m2 )
= 89,375 N (20,000 lbf)
(b) The maximum length to which the sample may be deformed without plastic deformation is determined
from Equations 6.2 and 6.5 as
&quot;
!%
li = l0 \$1 + '
#
E&amp;
&quot;
275 MPa %
= (115 mm) \$1 +
' = 115.28 mm (4.51 in.)
115 ! 10 3 MPa &amp;
#
6.22 Consider the brass alloy for which the stress-strain behavior is shown in Figure 6.12. A cylindrical
specimen of this material 6 mm (0.24 in.) in diameter and 50 mm (2 in.) long is pulled in tension with a force of
5000 N (1125 lbf). If it is known that this alloy has a Poisson's ratio of 0.30, compute: (a) the specimen elongation,
and (b) the reduction in specimen diameter.
Solution
(a) This portion of the problem asks that we compute the elongation of the brass specimen. The first
calculation necessary is that of the applied stress using Equation 6.1, as
! =
F
=
A0
F
#d &amp;
&quot;% 0 (
\$2'
2
=
5000 N
2
10*3 m &amp;
#6 )
&quot;%
2
\$
= 177!) !10 6 N/m2 = 177!MPa (25,000 psi)
(
'
From the stress-strain plot in Figure 6.12, this stress corresponds to a strain of about 2.0 &times; 10-3. From the definition
of strain, Equation 6.2
!l = &quot; l0 = (2.0 # 10 -3 ) (50 mm) = 0.10 mm (4 # 10 -3 in.)
(b) In order to determine the reduction in diameter ∆d, it is necessary to use Equation 6.8 and the definition
of lateral strain (i.e., ε = ∆d/d ) as follows
x
0
!d = d0&quot;x = # d0 \$ &quot; z = # (6 mm)(0.30) (2.0 % 10 -3 )
= –3.6 &times; 10-3 mm (–1.4 &times; 10-4 in.)
6.29 A cylindrical specimen of aluminum having a diameter of 0.505 in. (12.8 mm) and a gauge length of
2.000 in. (50.800 mm) is pulled in tension. Use the load–elongation characteristics tabulated below to complete
parts (a) through (f).
Length
N
lbf
mm
in.
0
0
50.800
2.000
7,330
1,650
50.851
2.002
15,100
3,400
50.902
2.004
23,100
5,200
50.952
2.006
30,400
6,850
51.003
2.008
34,400
7,750
51.054
2.010
38,400
8,650
51.308
2.020
41,300
9,300
51.816
2.040
44,800
10,100
52.832
2.080
46,200
10,400
53.848
2.120
47,300
10,650
54.864
2.160
47,500
10,700
55.880
2.200
46,100
10,400
56.896
2.240
44,800
10,100
57.658
2.270
42,600
9,600
58.420
2.300
36,400
8,200
59.182
2.330
Fracture
(a) Plot the data as engineering stress versus engineering strain.
(b) Compute the modulus of elasticity.
(c) Determine the yield strength at a strain offset of 0.002.
(d) Determine the tensile strength of this alloy.
(e) What is the approximate ductility, in percent elongation?
(f) Compute the modulus of resilience.
Solution
This problem calls for us to make a stress-strain plot for aluminum, given its tensile load-length data, and
then to determine some of its mechanical characteristics.
(a) The data are plotted below on two plots: the first corresponds to the entire stress-strain curve, while for
the second, the curve extends to just beyond the elastic region of deformation.
(b) The elastic modulus is the slope in the linear elastic region (Equation 6.10) as
E =
! &quot; 200 MPa \$ 0 MPa
=
= 62.5 % 10 3 MPa = 62.5 GPa (9.1 % 10 6 psi)
!#
0.0032 \$ 0
(c) For the yield strength, the 0.002 strain offset line is drawn dashed. It intersects the stress-strain curve at
approximately 285 MPa (41,000 psi ).
(d) The tensile strength is approximately 370 MPa (54,000 psi), corresponding to the maximum stress on
the complete stress-strain plot.
(e) The ductility, in percent elongation, is just the plastic strain at fracture, multiplied by one-hundred. The
total fracture strain at fracture is 0.165; subtracting out the elastic strain (which is about 0.005) leaves a plastic
strain of 0.160. Thus, the ductility is about 16%EL.
(f) From Equation 6.14, the modulus of resilience is just
Ur =
! 2y
2E
which, using data computed above gives a value of
Ur =
(285 MPa) 2
= 0.65 MN/m2 = 0.65 ! 10 6 N/m2 = 6.5 ! 10 5 J/m3
(2) (62.5 ! 10 3 MPa)
(93.8
in.- lb f /in.3)
6.41 Using the data in Problem 6.28 and Equations 6.15, 6.16, and 6.18a, generate a true stress–true
strain plot for aluminum. Equation 6.18a becomes invalid past the point at which necking begins; therefore,
measured diameters are given below for the last four data points, which should be used in true stress computations.
Length
Diameter
N
lbf
mm
in.
mm
in.
46,100
10,400
56.896
2.240
11.71
0.461
42,400
10,100
57.658
2.270
10.95
0.431
42,600
9,600
58.420
2.300
10.62
0.418
36,400
8,200
59.182
2.330
9.40
0.370
Solution
These true stress-strain data are plotted below.
6.44 The following true stresses produce the corresponding true plastic strains for a brass alloy:
True Stress (psi)
True Strain
50,000
0.10
60,000
0.20
What true stress is necessary to produce a true plastic strain of 0.25?
Solution
For this problem, we are given two values of εT and σT, from which we are asked to calculate the true
stress which produces a true plastic strain of 0.25. Employing Equation 6.19, we may set up two simultaneous
equations with two unknowns (the unknowns being K and n), as
log (50,000 psi) = log K + n log (0.10)
log (60,000 psi) = log K + n log (0.20)
Solving for n from these two expressions yields
n=
log (50,000) ! log (60,000)
= 0.263
log (0.10) ! log (0.20)
and for K
log K = 4.96 or K = 104.96 = 91,623 psi
Thus, for εT = 0.25
! T = K (&quot;T ) n = (91, 623 psi)(0.25) 0.263 = 63,700 psi
(440 MPa)
```